1 / 60

720 likes | 838 Vues

AMR - APARD. CEMENT CONCRETE MIX DESIGN. Dr.K.Lakshmi pathi Centre Head –CRIM AMR-APARD. DEFINITION.

Télécharger la présentation
## CEMENT CONCRETE MIX DESIGN

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.
Content is provided to you AS IS for your information and personal use only.
Download presentation by click this link.
While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
During download, if you can't get a presentation, the file might be deleted by the publisher.

E N D

**AMR - APARD**CEMENT CONCRETE MIX DESIGN Dr.K.Lakshmi pathi Centre Head –CRIM AMR-APARD**DEFINITION**• The process of selecting suitable ingredients of concrete and determining their relative quantities with the objective of producing a concrete of the required strength, durability, and workability as economically as possible, is termed the concrete mix design**Types of Mixes**• Nominal Mixes • In the past the specifications for concrete prescribed the proportions of cement, fine and coarse aggregates. These mixes of fixed cement-aggregate ratio which ensures adequate strength are termed nominal mixes. These offer simplicity and under normal circumstances, have a margin of strength above that specified. However, due to the variability of mix ingredients the nominal concrete for a given workability varies widely in strength**Nominal mix concrete**• Traditional way of mix proportion specified in terms of fixed ratios of Cement : Sand : coarse aggregate (In general by volume) • Useful for small works • Useful for routine concrete construction • Limited up to M20 grade • Requires high cement content C502.5**Standard mixes**The nominal mixes of fixed cement-aggregate ratio (by volume) vary widely in strength and may result in under- or over-rich mixes. For this reason, the minimum compressive strength has been included in many specifications. These mixes are termed standard mixes.**IS 456-2000 has designated the concrete mixes into a number**of grades as M10, M15, M20, M25, M30, M35 and M40. In this designation the letter M refers to the mix and the number to the specified 28 day cube strength of mix in N/mm2. The mixes of grades M10, M15, M20 and M25 correspond approximately to the mix proportions (1:3:6), (1:2:4), (1:1.5:3) and (1:1:2) respectively.**Designed Mixes**• In these mixes the performance of the concrete is specified by the designer but the mix proportions are determined by the producer of concrete, except that the minimum cement content can be laid down. This is most rational approach to the selection of mix proportions with specific materials in mind possessing more or less unique characteristics.**DESIGN MIX CONCRETE**• Several methods of mix design evolved over the years in different countries Ex: ACI practice, British practice, Indian Standard recommendations. etc.**Recommendations for concrete mix design are given in**• I.S.10262-1982 & I.S.10262-2009 • S.P.-23-1982 • Designed mix should meet the design requirements in the fresh and hardened states**Factors affecting the choice of mix proportions**• The various factors affecting the mix design are: • 1.Compressive strength • It is one of the most important properties of concrete and influences many other describable properties of the hardened concrete. The mean compressive strength required at a specific age, usually 28 days, determines the nominal water-cement ratio of the mix. The other factor affecting the strength of concrete at a given age and cured at a prescribed temperature is the degree of compaction. According to Abraham’s law the strength of fully compacted concrete is inversely proportional to the water-cement ratio.**2.Workability**• The degree of workability required depends on three factors. These are the size of the section to be concreted, the amount of reinforcement, and the method of compaction to be used. For the narrow and complicated section with numerous corners or inaccessible parts, the concrete must have a high workability so that full compaction can be achieved with a reasonable amount of effort. This also applies to the embedded steel sections. The desired workability depends on the compacting equipment available at the site.**3.Durability**• The durability of concrete is its resistance to the aggressive environmental conditions. High strength concrete is generally more durable than low strength concrete. In the situations when the high strength is not necessary but the conditions of exposure are such that high durability is vital, the durability requirement will determine the water-cement ratio to be used.**4.Maximum nominal size of aggregate**• In general, larger the maximum size of aggregate, smaller is the cement requirement for a particular water-cement ratio, because the workability of concrete increases with increase in maximum size of the aggregate. However, the compressive strength tends to increase with the decrease in size of aggregate. • IS 456:2000 and IS 1343:1980 recommend that the nominal size of the aggregate should be as large as possible.**5.Grading and type of aggregate**• The grading of aggregate influences the mix proportions for a specified workability and water-cement ratio. Coarser the grading leaner will be mix which can be used. Very lean mix is not desirable since it does not contain enough finer material to make the concrete cohesive. • The type of aggregate influences strongly the aggregate-cement ratio for the desired workability and stipulated water cement ratio. An important feature of a satisfactory aggregate is the uniformity of the grading which can be achieved by mixing different size fractions.**6.Quality Control**• The degree of control can be estimated statistically by the variations in test results. The variation in strength results from the variations in the properties of the mix ingredients and lack of control of accuracy in batching, mixing, placing, curing and testing. The lower the difference between the mean and minimum strengths of the mix lower will be the cement-content required. The factor controlling this difference is termed as quality control.**Mix Proportion designations**• The common method of expressing the proportions of ingredients of a concrete mix is in the terms of parts or ratios of cement, fine and coarse aggregates. For e.g., a concrete mix of proportions 1:2:4 means that cement, fine and coarse aggregate are in the ratio 1:2:4 or the mix contains one part of cement, two parts of fine aggregate and four parts of coarse aggregate. The proportions are either by volume or by mass. The water-cement ratio is usually expressed in mass**Factors to be considered for mix design**• The grade designation giving the characteristic strength requirement of concrete. • The type of cement influences the rate of development of compressive strength of concrete. • Maximum nominal size of aggregates to be used in concrete may be as large as possible within the limits prescribed by IS 456:2000. • The cement content is to be limited from shrinkage, cracking and creep. • The workability of concrete for satisfactory placing and compaction is related to the size and shape of section, quantity and spacing of reinforcement and technique used for transportation, placing and compaction.**procedure**• Target strength for mean strength The target mean compressive strength at 28 days (ft) =fck+ K.S K = a statistical value , usually taken as 1.65 S = standard deviation for each grade of concrete ( table 8 of I.S. 456 -2000 ) C502.6**Table-8, IS Code**C502.6**2.Selection of water cement ratio:**• A) The free water cement ratio corresponding to the target strength is to be determined from the graph shown in fig. C502.6**B) The water cement ratio, as selected above should be**checked against the limiting watercement ratio for the durability requirements as given in table**Durability Criteria as per IS 456- 2000**Adjustments to minimum cement content for aggregates other than 20 mm nominal max. size aggregates as per IS 456: 2000.**Approximate water content (Kg) per cubic metre of**concrete (Table 32, SP:23-1982)**3.Estimation of entrapped air**• Depends on nominal max size of aggregate as given in table C502.6**4.Selection of water content and fine to total aggregate**ratio • The values are given in the tables, based on the following conditions (a) Crushed (Angular) Coarse aggregate conforming to IS: 383 (b) Sand conforming to grading zone II of table 4 of IS 383 (c) Workability corresponds to C.F. of 0.8 C502.6**5.a. Approximate sand and water contents per cu.m of**concrete W/C = 0.6, Workability = 0.8 C.F. (For medium strength concrete up to M35) C502.6**Step 5 - Estimation of Coarse Aggregate Proportion**■ For W/C ratio of 0.5 use following Table**Correction in Coarse Aggregate values The table specified**for W/C ratio of 0.5 1. For Every +0.05 change in W/C ratio: -0.01 2. For Every -0.05 change in W/C ratio: +0.01 3. For Pumpable Mix : -10 % 57**5.c. Adjustments of values in Water Content and sand %**for other conditions C502.6**6.Determination of cement content**• a) From free W/C ratio and • b) quantity water per unit volume of concrete for workability (as derived in 5.c) Cement by mass = (Water content) / (w.c.r.) • This cement content should not be less than minimum content from the aspect of durability (given in 2.b) C502.6**where V = absolute volume of concrete**• = gross volume (1m3) minus the volume of entrapped air • Sc = specific gravity of cement • W = Mass of water per cubic metre of concrete, kg • C = mass of cement per cubic metre of concrete, kg • p = ratio of fine aggregate to total aggregate by absolute volume • fa, Ca = total masses of fine and coarse aggregates, per cubic metre of concrete, respectively, kg, and • Sfa, Sca = specific gravities of saturated surface dry fine and coarse aggregates, respectively**9. Determine the concrete mix proportions for the first**trial mix. • 10. Prepare the concrete using the calculated proportions and cast three cubes of 150 mm size and test them wet after 28-days moist curing and check for the strength. • 11. Prepare trial mixes with suitable adjustments till the final mix proportions are arrived at.**So the mix proportion works out to be**W : C : fa : ca = 185 : 411 : 635 : 1150 = 0.45 : 1 : 1.55 : 2.80 This mix will be considered as Trial Mix No.2**Step VII:- Make slump trials to find out the actual weight**of water to get required slump. Make corrections to the water content & %FA, if required. • Step VIII:- Compute 2 more trial mixes with W/C ratios as 0.40 & 0.50, taking %FA as 34% and 38% respectively.**Trial Mix No. 1:-**Cement = 185 / 0.4 = 462.5 Kg. Substituting the values in Eq(1), we get 1000 = 185 + 462.5/3.0 + (1/0.34) * fa /2.6) fa = 584 Kg. Substituting the values in Eq(2), we get 1000 = 185 + 462.5/3.0 + (1/0.66) * ca /2.65) ca = 1156 Kg. So the mix proportion works out to be W : C : fa : ca = 185 : 462.5 : 584 : 1156 = 0.4 : 1 : 1.26 : 2.50**Trial Mix No. 3:-**Cement = 185 / 0.5 = 370 Kg. Substituting the values in Eq(1), we get 1000 = 185 + 370/3.0 + (1/0.38) * fa /2.6) fa = 683 Kg. Substituting the values in Eq(2), we get 1000 = 185 + 370/3.0 + (1/0.62) * ca /2.65) ca = 1136 Kg. So the mix proportion works out to be W : C : fa : ca = 185 : 370 : 683 : 1136 = 0.5 : 1 : 1.85 : 3.07**Step IX:- Cast atleast 3 cubes for each trial mix.**• Step X:- Test the cubes for compressive strength at 28 days.**Step XI:- Draw a graph between compressive strength Vs C/W**Ratio.**Step XII:- From the graph, find the W/C ratio for the**required target mean compressive strength. • Step XIII:- Calculate the mix proportions corresponding to the W/C ratio, obtained from the graph.**Final Mix:-**From the graph, for a target strength of 390 Kg/Cm2, W/C ratio = 0.47 Cement = 185 / 0.47 = 394 Kg. Substituting the values in Eq(1), we get 1000 = 185 + 394/3.0 + (1/0.38) * fa /2.6) fa = 675 Kg. Substituting the values in Eq(2), we get 1000 = 185 + 394/3.0 + (1/0.62) * ca /2.65) ca = 1123 Kg. So the mix proportion works out to be W : C : fa : ca = 185 : 394 : 675 : 1123 = 0.47 : 1 : 1.71 : 2.85**Step XIV:- Check the cement content & W/C ratio against the**limiting values given in Table-5 of I.S: 456-2000 for given type of exposure & type of Concrete.

More Related